## A Definition of the Magnetic Transition

## Temperature Using Valence Bond Theory

### Joaquim Jornet-Somoza,

∗,†,‡### Mercè Deumal,

†### Juan Borge,

‡### and Michael A. Robb

¶†Departament de Ciència de Materials i Química Física and IQTCUB, Facultat de Química, Universitat de Barcelona, Martí i Franquès 1, E-08028 Barcelona

‡Nano-Bio Spectroscopy Group and ETSF Scientific Development Centre, Department of Materials Physics, University of the Basque Country, CFM CSIC-UPV/EHU-MPC and

DIPC, Tolosa Hiribidea 72, E-20018 Donostia-San Sebastián

¶Department of Chemistry, Imperial College London, South Kensington Campus, SW7 2AZ London

Abstract

Macroscopic magnetic properties are analyzed using Valence Bond theory.

Com-monly the critical temperature T_{C} for magnetic systems is associated with a maximum
in the energy-based heat capacity Cp(T ). Here a more broadly applicable definition of

the magnetic transition temperature T_{C} is described using spin moment expectation
value (i.e. applying the spin exchange density operator) instead of energy. Namely,

the magnetic capacity Cs(T ) reflects variation in the spin multiplicity as a function of

temperature, which is shown to be related to ∂[χT (T )]/∂T . Magnetic capacity C_{s}(T )
depends on long-range spin interactions that are not relevant in the energy-based heat
capacity C_{p}(T ). Differences between Cs(T ) and Cp(T ) are shown to be due to spin

order/disorder within the crystal, that can be monitored via a Valence Bond analysis

of the corresponding magnetic wavefunction. Indeed the concept of the Boltzmann spin-alignment order is used to provide information about the spin correlation between

magnetic units. As a final illustration, the critical temperature is derived from the

magnetic capacity for several molecular magnets presenting different magnetic topolo-gies that have been experimentally studied. A systematic shift between the transition

temperatures associated with Cs(T ) and Cp(T ) is observed. It is demonstrated that

this shift can be attributed to the loss of long-range spin correlation. This suggests
that the magnetic capacity C_{s}(T ) can be used as a predictive tool for the magnetic
topology, and thus for the synthetic chemists.

### Introduction

The first attempts to understand magnetism at the atomic level were carried out by Langevin
and Weiss using semiempirical theories. In 1905, Langevin1,2 _{provided a good description}

of paramagnetism for an atom or molecular magnet that carried a permanent magnetic moment, whose spatial distribution was to be given by the Boltzmann factor. In 1907, Weiss3predicted the existence of the Curie point (TC) below which ferromagnetism sets in by

means of introducing the effect of an internal or molecular field proportional to the intensity of magnetization. Later on, in 1913, the angular momentum was quantized and, hence, the magnetic moment of an atom or a molecule-based magnet using Bohr’s quantum theory,4

which employed classical mechanics combined with quantum conditions. This resulting in the definition of the magnetic susceptibility expressed by the Langevin-Debye formula,

χ(T ) = NAµ

2 B

3kBT

µ2_{ef f} (1)

where µef f and µB is the effective magnetic moment and Bohr magneton respectively, NA

is the Avogadro number, kB is the Boltzmann constant, and T the temperature of the

system. In 1927, Van Vleck5 _{established the general formula for the magnetic susceptibility}

using quantum mechanics for the zero external magnetic field limiting case. Van Vleck also
introduced the temperature dependence of the magnetic moment (µ).5 _{For the computation}

of µ it was necessary to know the energy of all stationary states of the system, En, to compute

the magnetic susceptibility. With the quantum derivation of Van Vleck, the magnetism of many atoms, molecules and compounds could be well described and their magnetic behavior could be also characterized as antiferromagnetic (AFM), ferromagnetic (FM) or diamagnetic, as a function of the microscopic magnetic interaction (Jij) between the spins i and j. The

Jij values are obtained from fitting the magnetic susceptibility curve to a given model6 or

computed using quantum chemistry tools.7,8

the spin-carrying units within the crystal. The relative alignment of two interacting S = 1/2 radicals generates three cases: (1) a FM interaction, when the spins of both radicals are coupled parallel to generate a triplet; (2) an AFM interaction, when the adjacent spins are coupled antiparallel to form a singlet; and (3) a paramagnetic behavior, when the unpaired spins show no magnetic interaction between them. In the case of many centers, the FM and AFM cases give rise to two limiting cases: (1) all adjacent spins are parallel to each other (which generates a bulk ferromagnet, when the FM interactions extend over the three directions of space), and (2) all adjacent spins are antiparallel (which results in a bulk antiferromagnet, when the AFM interactions extend over the three directions of space). Note that a particular case of antiferromagnetism is diamagnetism. Diamagnetism results from antiparallel spin-pairing with no net spin momentum. In between these two extreme cases, there are other possible combinations, which include dominant FM or AFM behavior, such as metamagnetism, change in magnetic dimensionality, or spin-canting6

The formulation of the macroscopic magnetic properties including magnetic susceptibil-ity χ(T ), magnetization M (H), and heat capacsusceptibil-ity Cp(T ) can be formulated with quantum

mechanics using statistical mechanics.5 However, the definition of the critical temperature TC below which the magnetic systems order and behave as FM, AFM, etc. is not completely

clear. A maximum in the heat capacity Cp(T ) is usually taken to indicate a second order

phase transition.9,10 _{However, this transition does not correspond to the appropriate }

mag-netic order/disorder physical transition, since it is associated with changes in energy, and not with changes in spin. Thus it is not the most suitable critical temperature for magnetism.

In 1962, Fisher11suggested that there was a correlation between a Cp(T ) and ∂[χT (T )]/∂T ,

implying that both had a similar physical interpretation.12–15 In this paper, we propose a definition of the magnetic critical temperature derived in the same way as Cp(T ), but using

the spin moment rather than the energy. We shall refer to this as the magnetic capacity Cs(T ). Cs(T ) is defined so that it accounts for the variation of the mean value of the spin

can be obtained directly from experimental data and is proportional to the magnetic capacity, Cs(T ). With these definitions we can identify long-range order or the lack of it with those

cases where TC obtained from either ∂[χT (T )]/∂T or Cs(T ) agrees or not with TC defined

in terms of Cp(T ).

In order to develop the main ideas related to the magnetic capacity Cs(T ), we will present

the mathematical expressions for macroscopic magnetic properties using Valence Bond the-ory. We show that the spin exchange density matrix operator in Valence Bond theory, which describes the bonding interaction, is also useful for the microscopic interpretation of the different magnetic observables. The expressions of Cs(T ) and Cp(T ) will be given using spin

exchange density matrix elements, Pij.16,17 It will be shown that the heat capacity Cp(T )

involves the derivative of the energy, whereas Cs(T ) involves changes on the spin moment.

The theoretical development and discussion of this paper is structured as follows. We start with the usual derivation of the macroscopic magnetic properties from statistical mechan-ics, and then present these very same magnetic properties using the spin exchange density matrix elements Pij. This gives rise to the definition of the magnetic capacity, Cs(T ). The

physical insight from this reformulation will then be discussed. Next we will discuss the in-terpretation of the magnetic capacity, in terms of the Valence Bond magnetic wavefunction, using the exchange density matrix (Pij terms). This reformulation allows the interpretation

of magnetic phenomena in terms of short- and long-range spin couplings.18 _{Such short- and}

long-range effects explain the differences between Cp(T ) and ∂[χT (T )]/∂T . Finally, we will

illustrate the application of the definition of TC defined in terms of Cs(T ) for the description

of magnetic critical temperatures of some molecular magnets that have been characterized experimentally.

### Theory

In this section, we first derive the magnetic properties χ(T ), Cp(T ) and Cs(T ) using a

description of the magnetic wavefunction obtained from Valence Bond theory. This in turn allows the definition of the Boltzmann magnetic spin-alignment order (˜µij), which describes

the temperature dependent spin-correlation between two radical centers (i and j). Then, an illustrative example is presented using a model linear system consisting in 4 spin-carrying S = 1/2 radicals with nearest-neighbor magnetic interactions (hereafter 4s model). In general, a ’ns’ model stands for the number ’n’ of radicals in the model and for ’s’ S = 1/2 unpaired spins.

Within the framework of molecule-based magnets, the magnetic susceptibility, χ, and heat capacity, Cp, are the macroscopic magnetic properties defining the temperature at which

the magnetic second order phase transition occurs, i.e. the magnetic transition temperature. Equations (2) and (3) show the theoretical expressions for the magnetic susceptibility χ(T ), and heat capacity Cp(T ) in absence of orbital angular momentum, developed by Van Vleck

in terms of the properties of each microstate,

χ(T ) = NAg
2_{µ}2
B
3kBT
X
n
Sn(Sn+ 1)(2Sn+ 1)e−En/kBT
P
n0(2Sn0 + 1)e−En0/kBT (2)
Cp(T ) =
NA
kBT2
P
nE
2
n(2Sn+ 1)e−En/kBT
P
n0(2S_{n}0 + 1)e−En0/kBT −
P
nEn(2Sn+ 1)e
−En/kBT2
P
n0(2S_{n}0 + 1)e−En0/kBT2
(3)
where g and µB are the gyromagnetic constant and Bohr magneton respectively, and En and

Sn are the energy and spin multiplicity of the n microstate. From these expressions, we can

see that the energy and spin multiplicity of the n microstates are the only quantities that depend directly on the system and give the magnetic properties in equations (2) and (3).

In previous work, we have shown that these magnetic microstates can be obtained by solving an algebraic eigenvalue problem associated with a Heisenberg Hamiltonian for spin 1/2 particles,19

ˆ

H = −2X

i,j

JijSˆiSˆj (4)

where ˆSi is the spin operator acting on center i, and Jij is the microscopic magnetic

inter-action between spin centers i and j. As written, the Hamiltonian acts on a space of neutral covalent Slater determinants where each orbital i occurs only once with either α or β spin. Thus the operators ˆSi operate on the spin of orbital i. The Jij are the exchange integrals of

Heitler-London Valence Bond theory (for a model two-electron system with orbitals i and j). The Jij can be obtained from ab initio computations on a pair of radicals.20 See Supporting

Information Section 1 for a discussion on the working strategy followed to bring together Jij

and macroscopic magnetic properties.

Equation (4) corresponds to a model Hamiltonian with computed parameters that reduces the problem of chemical binding to coupling of electron spins. Anderson21 was the first to recognize that Heisenberg Hamiltonians might be understood as effective Hamiltonians computed from an exact full configuration interaction (CI) Hamiltonian using a model space of neutral Valence Bond determinants formed from n electrons in n atomic orbitals. The use of such spaces in quantum chemistry was first proposed in this context by Malrieu and co-workers.16,22–25

Our implementation of a Heisenberg Hamiltonian model has been used to study mag-netic interactions in many problems.26–32 In order to keep this paper self-contained, before reformulating equations (2) and (3), we will briefly review some essential aspects of the Heisenberg spin Hamiltonian (equation 4) and how it can be used to study magnetic prop-erties of molecule-based magnets.

Traditionally, Valence Bond theory, formulated as a Heisenberg Spin Hamiltonian, is based on the use of localized active orbitals. One uses a neutral covalent determinant basis [ΦK, ..., ΦL] in which each orbital occurs at most once with α or β spin (see Supporting

electrons). The orbitals are assumed to be non-orthogonal of the Coulson-Fischer type.33,34 However, the orthogonality is reflected on the parametrization of the Jij and the orbitals are

never treated explicitly.35

Lets now define the spin-exchange operator ˆPij as permutation operator that interchange

the spin coordinate of two electrons. For example, the application of the spin-exchange operator over four 2 electrons spin primitive functions, leads to:

ˆ P12α(1)α(2) = α(1)α(2) ˆ P12α(1)β(2) = β(1)α(2) ˆ P12β(1)α(2) = α(1)β(2) ˆ P12β(1)β(2) = β(1)β(2) (5)

Then, we can construct a certain operator using the spin permutation that has the same effect as the spin operator product ( ˆSi· ˆSj) presents in the Heisenberg Hamiltonian (equation

4). This is the so called Dirac identity,17 which in the case of two spins is [ ˆS(1) ˆS(2)]Θ(1, 2) = −1 2 ˆ P12− 1 4 ˆ IΘ(1, 2) (6) i.e. P12= D − 2[ ˆS(1) ˆS(2)] + 1 2Iˆ E (7) where Θ(1, 2) is any two-electron spin function, and ˆI is the identity operator. The spin-exchange density matrix Pij is a useful analytic concept, which matrix elements are computed

as the expectation values of ˆPij (equation 7). These can be defined, using the general

expression of a two electron operator in second quantization,36 as hΨ| ˆPij|Ψi = − X i,j,k,l hi(1)j(2)| ˆS(1) ˆS(2) + 1 4 ˆ

I(1, 2)|k(1)l(2)i × hΨ|a†_{i}a†_{j}alak|Ψi (8)

integration of the spatial part gives Kronecker-δ terms, and by resolving the spin operator using step-up and step-down operators, we obtain the final expression:37

Pij = Pijαβ − P
αα
ij (9a)
P_{ij}αβ = 1
2hΨ|a
†
iαajαa
†
jβaiβ+ a
†
iβajβa
†
jαaiα|Ψi (9b)
P_{ij}αα = 1
2hΨ|a
†
iαa
†

jαajαaiα+ a†_{iβ}a†_{jβ}ajβaiβ|Ψi (9c)

One can see that the exchange density matrix Pij elements are the difference between

exchange terms for electrons of different P_{ij}αβ and same Pαα

ij spin, respectively. In general

Pij can be obtained in terms of the coefficients of the expansion of the multiconfigurational

magnetic wavefunction, as:

P_{ij}αβ = 1
2
X
K,L
cKcLhΦK|a
†
iαajαa
†
jβaiβ|ΦLi (10a)
P_{ij}αα = 1
2
X
K
c2_{K}hΦK|a
†
iαa
†
jαajαaiα|ΦKi (10b)

The Pij terms are just a two-particle density matrix elements that can be obtained from

any CI computation.37 _{For wavefunctions composed of several Valence Bond structures, the}

values of Pij give a quantitative measure of the bonding, as suggested early by Penney and

Moffitt.38 Further, the spin-exchange density matrix elements are related to the total spin by:17 S(S + 1) = −N (N − 4) 4 − X i<j Pij, (11)

where N is the number of unpaired electrons. Notice that equation (11) can be used to com-pute the spin multiplicity of each of the multiconfigurational eigenfunctions of the Heisenberg Hamiltonian.

as:18 ˆ H = −X ij Jij(2 ˆSiSˆj + 1 2 ˆ I) =X ij JijPˆij (12)

where the expectation values of both Hamiltonians (equations 4 and 12) are related by a shift due to the identity operator. Further, one can see that the energy spectrum can be also obtained using,

∆En =

X

i<j

Jij∆Pijn, (13)

where ∆En = En− E0 and ∆Pijn refer to the differences of the energy values and Pij matrix

elements between the nth _{excited state and the ground state, respectively.}

As mentioned above, the exchange density matrix elements Pij are related to the relative

alignment of the spin of electrons in magnetic centers i and j. For a two-electron system (N = 2, 2s model) with spins either coupled antiparallel or parallel or uncoupled, the reference Pij values are given in Figure 1. For S = 0 (Figure 1a), h ˆS(i) ˆS(j)i = −3/4 and the Pij

element has a value of +1.0 , while if coupled parallel S = 1 (Figure 1b), h ˆS(i) ˆS(j)i = +1/4
and the Pij will be -1.0 . In addition, for uncoupled spins, hS2i = 2[1_{2}(1_{2} + 1)] = +3/2 and

h ˆS(i) ˆS(j)i = 0, the value of the corresponding Pij element is -0.5 (see Figure 1c). For that

reason, from a VB perspective, Pij can be suitably denoted as magnetic bond-order

(µ-BO). We have given some discussion of physical interpretation of the spin exchange density matrix elements in the Supporting Information Section 3. There we give the Pij for the

Kekulé and Dewar VB structures of the π-electrons of the benzene molecule.

We now discuss the temperature dependence into the magnetic properties using statistical mechanics of the canonical ensemble. In such scheme, the population of each microstate (n) is defined by the Boltzmann distribution function, fn

B(T ) =

(2Sn+1)

Z e

−En/kBT_{, where Z stands}

(a) antiparallel spin alignment Pij = +1 (b) parallel spin alignment Pij = -1 (c) non-ordered spin alignment Pij = -0.5

Figure 1: Relative alignment of the spin of electrons in magnetic centers i and j for a two-electron system (2s): (a) antiparallel, (b) parallel, and (c) non-ordered or uncoupled. The Pij values are also given from equation (11).

the microstate n. Therefore, the temperature dependent expectation values of the spin multiplicity and energy can now be expressed in terms of the eigenvalues of the Heisenberg Hamiltonian equation (12), i.e. the spin multiplicity and energy of each microstate. Using equations (11) and (13), these hEiT and hS2iT expectation values can be expressed in terms

of the spin exchange density matrix elements,

hEiT =
X
n
∆En· fBn(T ) =
X
n
X
i<j
Jij∆Pijn· f
n
B(T ), (14)
hS2_{i}
T =
X
n
Sn(Sn+ 1) · fBn(T ) = −
N/(N − 4)
4 −
X
n
X
i<j
P_{ij}n· fn
B(T ), (15)

Now we can define the temperature dependent spin-alignment order matrix, ˜µ(T ) . The elements of ˜µ(T ) between two spin carrying units i and j are defined as the Boltzmann weighted spin exchange density matrix element,

˜
µij(T ) =
X
n
P_{ij}n· fn
B(T ). (16)

This Boltzmann weighted magnetic bond-order matrix carries information about the correlated alignment between all the spin units and its temperature behavior. We shall refer to ˜µ(T ) (equation 16) as Boltzmann magnetic µ-bond order. The macroscopic magnetic properties, in terms of the spin exchange density matrix elements, Pij , of each microstate

function of the temperature, we differentiate hEiT (equation 14) with respect to temperature.

Thus the magnetic capacity, Cs(T ), is obtained by differentiating hS2iT (equation 15) with

respect to temperature,
Cp(T ) =
∂hEiT
∂T =
NA
kBT
X
n
"
X
i<j
(Jij · Pijn(J ))
f_{B}n(T )
X
m
(Em− En)fBm(T )
#
, (17)
Cs(T ) =
∂hS2_{i}
T
∂T =
NA
kBT
X
n
"
X
i<j
(P_{ij}n(J ) + P_{ij}n(0))
f_{B}n(T )
X
m
(Em− En)fBm(T )
#
.
(18)
In equations (17) and (18), we have identified two types of spin-exchange density
ma-trix elements, Pij(J ) and Pij(0), which occur in the Heisenberg spin Hamiltonian energy

expression (equation 12). Pij(J ) corresponds to a Pij where the value of Jij is finite,

while Pij(0) corresponds to a Pij where the value of Jij is vanishingly small (in previous

calculations it was defined to be < |0.05|cm−1).19,39 _{Thus P}

ij(0) corresponds to the

long-range spin coupling that has no energetic effect in the Heisenberg Hamiltonian. Thus the Pij(J ) (and ˜µij(J, T )) elements are those where magnetic interaction Jij has a non-negligible

value, i.e. a connected/short-range spin alignment is present, while the terms labeled Pij(0)

(and ˜µij(0, T )) have Jij = 0 (hence it does not appear in equation (17)), and show a

non-bonded/long-range spin alignment. This classification turns out to be useful for understand-ing the physical phenomena that take place upon magnetic transition.

We now discuss some conceptual aspects of the two magnetic properties defined in equa-tions (17) and (18). The heat capacity Cp(T ) involves a change in the energy of the whole

system, and depends on the spin-alignment between the magnetic centers with non-negligible magnetic interactions, Pij(J ). The magnetic capacity Cs(T ) involves a change of the spin

moment of the whole system, and depends on the spin-alignment between all pairs of mag-netic centers, including those for which Jij is zero. This latter term includes the effect of

long-range spin ordering, as experimentally40,41 and theoretically18,42 suggested. The role of the Boltzmann magnetic µ-bond order and its relation with the spin-exchange density

matrix values Pij in equations (17) and (18) allows a simple relationship between structure

and magnetism. In addition, the maximum of the magnetic capacity function indicates an inflection point at which the long-range spin pairs start to be ordered when cooling from high to low temperature. In contrast, the maximum of the heat capacity describes the tran-sition at which the nearest-spins become correlated, i.e. the existence of a short-range spin ordering.

### Results and Discussion

### Conceptual Development

In this section we shall give some physical insight into the concepts presented in the previous section. This discussion has two facets. On the one hand we wish to demonstrate the effect of Pij(J ) and Pij(0) on Cs(T ) and Cp(T ) for a model 4 electron system (4s). Then we

shall discuss the relationship of the experimental quantity (∂[χT (T )]/∂T ) to either Cs(T ) or

Cp(T ), and analyze the effect of the magnetic topology.

We now illustrate the theoretical ideas just discussed using the Boltzmann magnetic µ-bond order for a four S = 1/2 radical system whose four unpaired electrons interact linearly (4s). The simplest magnetic model results from the interaction between two radical centers with one unpaired electron each (hereafter 2s model). However, this model is not adequate to illustrate the different physical meaning of the heat and the magnetic capacities since it does not have any long-range order Pij(0). Thus the simplest model we can use is formed

by four S = 1/2 magnetic units linearly interacting (4s). We also choose J = −50cm−1. We now illustrate the application of the magnetic wave function analysis in terms of Pij using the

4s AFM linear model (see Figure 2a for magnetic topology; and Figures 2b,c for short- and long-range spin alignment, respectively). As we will see bellow, the physical interpretation does not depend on the value of the magnetic interaction, but on the magnetic topology.

al-(a) (b) (c)

Figure 2: (a) Magnetic topology for a four-spin center 4s antiferromagnetic AFM linear model (J = −50cm−1 represented as straight red lines). (b) Schematic representation of the short-range spin exchange density matrix elements Pij(J ) (solid blue lines). (c) Schematic

representation of the long-range spin exchange density matrix elements Pij(0) (dashed brown

lines).

lows one to obtain the multiconfigurational magnetic wavefunctions of the ground and ex-cited states of our system (the authors strongly encourage interested readers to address to Supporting Information Section 4 for further details on the chemical analysis of the spin interactions using VB theory). Then, by applying equation (10), the magnetic bond order (µ-BO) for each spin-pair in each magnetic state can be computed. The individual computed Pij will differ from the ideal values shown in Figure 1 due to the multiconfigurational nature

of the magnetic wave function.

The µ-BO (i.e. the exchange density matrix element Pij) is indicative of the nature of the

relative alignment of the spin of electrons in magnetic centers i and j (see Figure 1 for a two-electron system). Then extending this idea by applying the corresponding Boltzmann factor, we can visualize the temperature evolution of the magnetic µ-bonds as shown in Figure 3a. In other words, the Boltzmann weighted Pij elements enable one to study the temperature

dependence of the magnetic µ-bond order, ˜µij(T ). Note that parallel spin alignment has

been assigned to Pij values ranging from -0.5 to -1.0, which are displayed in blue in Figure

3a. The antiparallel spins are attributed to Pij from -0.5 to +1.0 (shown in red in Figure

3a). The strength of the ˜µij(T ) representation increases (indicated by line thickness) as

the temperature decreases. This directly translates into an increase of the spin alignment correlation. Between 53-100 K it is possible to observe that the short-range spin ordering ˜

(a)

(b)

Figure 3: (a) Representation of ˜µij(J, T ) (upper) and ˜µij(0, T ) (lower) contributions at a

temperature of interest for the 4s linear AFM system. Notice that parallel (antiparallel) spin alignment is displayed in blue (red). (b) Representation of the magnetic capacity (Cs(T ),

Figure 3a. This in turn correlates with the maximum in Cp(T ) shown in Figure 3b. For the

long-range spin ordering or correlation ˜µij(0, T ) (i.e. hPij(0)iT), the actual strengthening

takes place between 36.5-53K, leading to the maximum in Cs(T ) shown in Figure 3b. From

Figure 3b one can see that, when cooling the system from high temperatures, the heat capacity Cp begins to increase at higher temperatures than the magnetic capacity Cs. If

one continues lowering the temperature, the maximum of the heat capacity can be observed around 53K. The magnetic capacity curve however displays its maximum value at ca. 36.5K. The central idea here is that the largest change of the spin moment of the whole system is accomplished at lower temperatures than the largest change of the energy of the whole system. In the following, we will explain the reason for this shift by simply using the definition of the ˜µij(T ), i.e. the fact that the new reformulation (equations 17 and 18)

implies Boltzmann factor weighted Pij terms.

0 50 100 150 200 250 Eigenstate Energy (cm−1) P ijPijn(0) P ijPijn(J )

Figure 4: Variation of the sum of spin-exchange density matrix elements (Pij) as a function

of the energy level for a 4s linear AFM chain. The different trend of all long-range Pij(0)

terms (red, sum over the Pij(0) elements) and short-range Pij(J ) terms (blue, sum over the

Pij(J ) elements) is represented for the six possible eigenstates.

From expressions (17) and (18), it is apparent that the different behavior of Cs(T ) and

Cp(T ) is directly related to the different Pij contributions (summation over the i, j spin

pairs). Figure 4 shows the variation of the sum of the Pij(0) and Pij(J ) elements for each

we see that the sum of all short-range Pij(J ) values linearly decreases as the energy of the

eigenstates increases, with slope equal to the magnetic interaction, Jij. In contrast, the sum

of all long-range Pij(0) terms changes/fluctuates between different states. Now, let us take

a look at equations (17) and (18). We can see that Cp(T ) is proportional to the sum of the

J -scaled Pij(J ) elements while Cs(T ) is proportional to the sum of all raw Pij elements. This

is the key-factor that governs the two different magnetic phase transitions.

The physical interpretation of this fact is easy to explain. By increasing the temperature, the magnetic excited states start to be populated and, in turn, all of the Pij values of each

state contribute on the magnetic ordering/disordering (see Supporting Information Section 4 for magnetic states). Since the long-range µ-bond orders, Pij(0), differ significantly between

excited states (Figure 4), the global long-range spin ordering tends to cancel out at lower temperatures. In other words, this description enables us to identify two physical processes: while Cp(T ) measures the short-range spin correlation, Cs(T ) will give information about

long-range correlation. As we shall presently discuss, when the above Boltzmann µ-bond order study is extended to real molecular magnets the conclusions reached were the same as for the 4s AFM chain model (see discussion on KAXHAS in Supporting Information Section 5).

Both Cp(T ) and Cs(T ) macroscopic properties allow the identification of a characteristic

temperature (TC) at which the system rapidly changes its behavior. In other words, for both

descriptions there exists a temperature at which the derivative of the energy or spin moment becomes zero, revealing critical phenomena. We have illustrated the different nature of the transition signaled by the heat capacity and magnetic capacity, Cp(T ) and Cs(T ) respectively.

Equations (17) and (18) show that the heat capacity Cp(T ) depends on the variation of the

Pij(J ) (short-range spin alignment), while the variation of both Pij(J ) and Pij(0)

(short-and long- range spin alignment, respectively) terms play an important role in determining the magnetic capacity Cs(T ) (see Figure 5). Note that all the analyses here performed have

conclusions are however not sensitive to the selected cut-off: (i) Cs(T ) would not be affected,

since it already considers all spin correlations; and (ii) Cp(T ) would be the property affected,

but since it is scaled by Jij itself it already accounts for the threshold chosen.

Figure 5: Flowchart connecting the heat capacity Cp(T ) with its source, which is the energy

distribution. Similarly, the magnetic capacity Cs(T ) is related to the spin moment.

As reported above, the magnetic capacity always reflects a critical temperature (T_{C}µ)
which is lower to the one found by the heat capacity (Th

C). This is due to the fact that,

for extended systems, and due to a thermal mixture of the magnetic microstates, the long-range magnetic ordering is always lost at lower temperatures than the short-long-range magnetic ordering. This statement demonstrates the complementarity role of both properties in order to properly characterize a magnetic material. Therefore, we can conclude that TC calculated

from either Cp(T ) or Cs(T ) will be nearly equal only in those molecule-based systems in

which the long- range spin correlation can be neglected, or there is no 3D propagation of the spin coupling.

Usually the magnetic transition is characterized following measurements of the heat
ca-pacity.10,12–15 _{However, it is often seen that this magnetic critical temperature can also be}

obtained measuring the first derivative of the magnetic susceptibility times the temperature (∂[χT (T )]/∂T ), which is known as Fisher’s heat capacity.12–15This name is adopted in

refer-ence to the direct proportionality suggested by Fisher,11and used to determine the magnetic ordering.43,44

We now discuss the relationship with Fisher’s heat capacity. If we compare the new magnetic capacity Cs(T ), formulated in equation (18), with the well-known expression (1)

for the magnetic susceptibility χ(T ), we notice that the effective magnetic moment µ2
ef f can
be replaced by:
χ(T ) = NAµ
2
B
3kBT
µ2_{ef f} = NAg
2_{µ}2
B
3kBT
hS2iT (19)

Notice that for a non-interacting spin system, whose simplest realization would involve a large energy separation between ground state and first excited states, the Boltzmann distribution can be neglected, and the effective magnetic moment (µef f) can be considered temperature

independent. However, equation (19) shows that temperature dependence has to be taken into account for general cases.

In this context it is clear that what we have defined as magnetic capacity Cs(T )) (equation

18) is directly proportional to the derivative of the magnetic susceptibility or Fisher’s heat capacity, ∂[χT (T )] ∂T = NAg2µ2B 3kB Cs(T ) (20)

As we have mentioned above, M.E. Fisher suggested a direct proportionality between Cp(T ) and χ(T ) observables, giving rise to the fact that both properties should exhibit the

same transition temperature. However, our derivation indicates that this proportionality is only accomplished when the magnetic crystal acts as a sum of isolated spin-pairs. In other words, for magnetic materials that can present long-range spin ordering, the critical temper-ature is no longer correlated with the maximum in Cp(T ) . Thus the magnetic capacity is

capable of identifying short- or long-range magnetic (µ-) bond order or magnetic correlation, which can easily be experimentally measured with the maximum in ∂[χT (T )]/∂T . There-fore, one can look in detail at the results of the calculations and understand the nature of the long/short range magnetic order in the crystal.

### Computed T

C### for several examples using C

s### (T ) and C

p### (T ) and

### com-parison with experimental maximum in (∂[χT (T )]/∂T ).

We now test the validity of the µ-bond order concept in magnetic structure calculations via the computation of TC for several examples using Cs(T ) and Cp(T ) and comparison

with experimental maximum in (∂[χT (T )]/∂T ). For simplicity we will use magnetic units
carrying spin 1/2 on a number of key prototypical molecular magnets (see column 1 in
Table 1).19,45–50 _{The analyzed molecular magnets are made by Cu(II)-based radicals, except}

for UBUBIC and KAXHAS, whose magnetism is due to purely organic radicals.51 For all these molecule-based magnets, good agreement between computed and experimental data was obtained for χ(T ) magnetic susceptibility and Cp(T ) heat capacity temperature response

curves using expressions (2) and (3), respectively (see Supporting Information Section 1 for more details on the first principles simulation working strategy). A variety of real magnetic topologies have been examined (column 2 in Table 1), including regular and alternating 1D chains, strong-rail and strong-rung spin-ladders, 2D AFM layer, 3D AFM interacting honeycomb layers and 3D FM diamond-type (see column 3 in Table 1 for most significant calculated Jij values).19,45–50

The maximum of ∂[χT (T )]/∂T , the so called Fisher’s heat capacity, has also been
ob-tained by numerical differentiation from experimental data (see column 4 for T_{C}∂[χT (T )]/∂T in
Table 1). The critical temperature of the magnetic capacity Cs(T ), namely TCµ, of seven

real systems has been calculated applying equation (18) (see column 5 in Table 1). Finally, simulated and experimental values for the critical temperature Th

C referring to Cp(T ), i.e.

the temperature at which the magnetic property exhibits a maximum, are compared (see
column 6 for T_{C}h).

The value of the maximum in ∂[χT (T )]/∂T is the experimental reference point. The value
of TC computed from Cs(T ) is in acceptable agreement with this value ( T_{C}µ≈ T_{C}∂[χT (T )]/∂T),

Table 1: Comparison between computed characteristic temperatures for seven studied prototypical crystals. CCDC name is given in column 1. Magnetic topology and significant Jij values (in cm−1 are given in columns 2 and 3.

Char-acteristic temperatures (in K) extracted from ∂[χT (T )]/∂T , magnetic capacity,
and heat capacity are given in columns 4-6. a _{% computed at calculated T}

C

as [Th

C(Cp) − TCµ(Cs)]/TCh(Cp) ∗ 100 . Note that Alt=Alternating; SP=spin-ladder;

exp=experimental; calc=calculated.
CCDC
name
magnetic
topology
Jij/cm−1
(calc)
Tc∂[χT ]/∂T
(exp)
Tµ
c(Cs)
(calc)
Te
c(Cp)
(exp/calc)
%(Cs/Cp)
(calc)a
CUPYAR45 1D Chain -5.23 4.31 5.60 5.22/6.85 18.2
UBUBIC46 1D Alt Chain -54.43/-55.97 74 60.20 –/72.60 17.1
TEXDEG47 Strong-rail SP -7.79/-3.49 6.50 6.35 –/9.20 31.0
XANKED48 _{Strong-rung SP} _{-13.82/-10.26} _{35.92} _{47.70} _{–/50.10} _{4.8}

CUPYZP49 _{2D Layer} _{-5.62} _{8.4} _{11.65} _{–/15.30} _{23.9}

GIVZOB50 _{3D Honeycomb} _{-8.21,-4.91/-2.44} _{6.1} _{6.40} _{–/7.75} _{17.4}

KAXHAS19 3D Bulk FM +0.68/+0.18 - 0.23 0.60/0.70 67.1

as expected from their direct relationship (see equation 20). The transition temperature T_{C}µ
is thus the most meaningful TC because it results from a magnetic spin transition, i.e. from

the thermal variation of the spin multiplicity of the system. T_{C}µ reflects the importance of
the non-connected spin alignment and the dominant effect of long-range spin correlation.
The difference between experimental and computed values has been demonstrated to be
mainly due to the variation of the crystal structure owed to the temperature at which it
has been determined.52 Further, if experimental T_{C}∂[χT (T )]/∂T and calculated T_{C}µ values are
very different it could also be an indication of the presence of impurities in the sample,
the existence of different crystal phases, or the simple presence of unanticipated magnetic
interactions because we make no assumptions in the simulation of χ(T ).

The non-constancy of the ratio between calculated Cs magnetic capacity and calculated

Cp heat capacity (see column 7 in Table 1) supports that there is no direct proportionality

between ∂[χT (T )]/∂T and Cp(T ). Therefore, Fisher’s suggestion is not applicable on real

to be extremely dependent on the magnetic topology of each molecular material.
There-fore, although this dependence is not the focus of this paper, this fact can be useful for
the experimental material science community to predict the magnetic dimensionality of a
molecule-based magnet of interest, and then use the appropriate analytical expressions to
obtain a fitted J parameter. The calculation of T_{C}µ(Cs) will thus enable one to estimate the

magnetic topology, and hence predict which is the best procedure to perform measurements as a function of the working temperature range, etc.

Finally, comparison between TC computed from Cs(T ) and Cp(T ) (both calculated

theo-retically) should give an indication of the effects of long-range order (indicated numerically (%) in column 7, Table 1). KAXHAS, which is a 3D bulk ferromagnet, has the largest (% TC Cs/Cp) value. This can be expected, since there are multiple ”short-range” paths to

connect long-range spin carrying units. Then a small fluctuation of the short-range align-ments (Pij(J )) will produce a small deviation on the total energy, but a large deviation of

the long-range spin correlation. In line with this argument, XANKED has the smallest (% TC Cs/Cp) value, which is also compatible with its magnetic topology being a strong rung

spin ladder. Since the spin-ladder has largest J(rung) interaction than J(rail), short-range spin correlation within a rung (i.e. between a 2 spin-carrying radicals, 2s model) has similar behavior as a 2s quasi-isolated topology. We can thus conclude that the discrepancy between TC computed from magnetic Cs(T ) and heat Cp(T ) capacities can be explained in terms of

the order in the crystal. It must be further emphasized that the systematic shift of the transition temperature computed from Cs(T ) and Cp(T ) (i.e. T

µ

C(Cs) < TCh(Cp))), which

was observed for the 4s model, is also realized for the seven real molecule-based magnets
here analyzed due to the different behavior of both short- and long-range spin correlations.
Note also that, even if the difference between T_{C}µ(Cs) and TCh(Cp) critical temperatures is

not very large, it can be of crucial importance when studying physical properties around the critical point.

### Conclusions

In this paper it is established that the heat capacity Cp(T ) measures the energy variation due

to the 3D propagation of the interaction of two magnetically connected spins, i.e. to short-range ordering. The magnetic capacity Cs(T ), in turn, is a measure of the thermal variation

of the spin multiplicity of the system, and reflects the importance of magnetically non-connected spin alignment and how the dominant effect of long-range spin correlation governs the magnetic behavior of molecule-based crystals (and in general of magnetic compounds).

We show that the current definition of the critical temperature TC for magnetic systems,

which is associated with a maximum in the heat capacity Cp(T ), does not capture the

magnetic nature because it excludes long-range magnetic order. Instead, a maximum in ∂[χT (T )]/∂T , that is related to the magnetic capacity Cs(T ) which in turn includes changes

in short- and long- range spin order/disorder, is a more broadly applicable definition of the magnetic transition temperature.

The magnetic capacity Cs(T ) is also useful because it can be interpreted in terms of

the molecular structure of the crystal using the magnetic wavefunction for each magnetic microstate. For this interpretation, we have used a Valence Bond analysis of the mag-netic wavefunction. This analysis uses the concept of the Boltzmann magmag-netic bond order (˜µ(T )), which is in turn defined using the exchange density matrix Pij. Whereas the

lat-ter provides information about the spin correlation between magnetic units, the Boltzmann magnetic µ-bond order elements, ˜µ(J, T ) and ˜µ(0, T ), are a very powerful tool to visualize the temperature-dependence of the magnetic correlation between all spin units.

After analysis of seven experimental magnetic systems, we demonstrate the existence of a systematic shift between the transition temperatures associated with Cs(T ) and Cp(T ) which

we demonstrate can be attributed to the loss of long-range spin correlation. We conclude that TC calculated from either Cp(T ) or Cs(T ) will be nearly equal only in those

molecule-based systems in which the long-range spin correlation can be neglected, or there is no 3D propagation of the spin coupling. This suggests that the magnetic capacity Cs(T ) can be

used as a predictive tool for the magnetic topology, and thus for the synthetic chemists. In addition, this type of analysis will enable further research to promote better understanding about what happens in the region close to the magnetic transition regime as a function of the magnetic topology.

### Acknowledgement

JJS and JB thank he European Research Council (ERC-2010-AdG-267374), Spanish grant (FIS2016-79464-P), and Grupos Consolidados (IT578-13) for the financial support. JJS gratefully acknowledges the Spanish grant IJCI-2014-22204. JB also acknowledges funding from the European Unions Horizon 2020 research and innovation program under the Marie Sklodowska-Curie Grant Agreement No. 703195. MD thanks the Spanish Government for financial support (projects MAT2008-02032/MAT and MAT2014-54025-P), and the Cata-lan DURSI (2005-SGR-0036 and 2014-SGR-1422). MD also acknowledges AGAUR for a travel grant (2007BE200188). We also acknowledge Prof. Mark M. Turnbull for fruitful discussions.

### Supporting Information Available

The following files are available free of charge.

• Detailed description of the bottom-up procedure used on the theoretical study of the magnetic properties (Section 1. Overview of the First-Principles Bottom-Up (FPBU) working strategy). Construction of a 4 electron paired Valence Bond basis set (Section 2: Paired Valence Bond function). Physical interpretation of the spin exchange density matrix elements of benzene resonant picture (Section 3: Valence Bond: Kekulé vs Dewar). Description and characterization of the multiconfigurational eigenstates of the 4s model (Section 4: Magnetic wavefunction decomposition (GS and ExS)). Boltzmann

µ-bond order study for the KAXHAS molecular magnet (Section 5: µ-Bond order analysis of KAXHAS crystal).

This material is available free of charge via the Internet at http://pubs.acs.org/.

### Notes and References

(1) Langevin, P. Magnetism and theory of electrons. Annales de Chimie et de Physique 1905, 5, 70–127.

(2) Langevin, P. Sur la théorie du magnétisme. Journal de Physique Théorique et Appliquée 1905, 4, 678–693.

(3) Weiss, P. L’hypothèse du champ moléculaire et la propriété ferromagnétique. J. Phys. Theor. Appl. 1907, 6, 661–690.

(4) Rosenfeld, L., Nielsen, J. R., Eds. EARLY WORK (1905-1911); Niels Bohr Collected Works; Elsevier, 1972; Vol. 1; pp 497–586.

(5) Van Vleck, J. In The International Series of Monographs on Physics; Flowler, R., Kapitza, P., Eds.; Oxford At The Clarendon Press, 1932; p 384pp.

(6) Kahn, O. Molecular Magnetism; VCH Publisher, Inc, 1993; p 380.

(7) Trinquier, G.; Suaud, N.; Guihéry, N.; Malrieu, J.-P. Designing Magnetic Organic Lat-tices from High-Spin Polycyclic Units. ChemPhysChem 2011, 12, 3020–3036.

(8) Mayhall, N. J.; Head-Gordon, M. Computational quantum chemistry for single Heisen-berg spin couplings made simple: Just one spin flip required. Journal of Chemical Physics 2014, 141 .

(9) Ivancevic, V. G.; Ivancevic, T. T. Springer Series: Understaning Complex Systems; Springer-Verlag Berlin Heidelberg, 2008; p 884.

(10) Carlin, R. L. Magnetochemistry; Springer-Verlag Berlin Heidelberg, 1986.

(11) Fisher, M. E. Relation between the specific heat and susceptibility of an antiferromag-net. Philosophical Magazine 1962, 7, 1731–1743.

(12) Wolf, W. P. Review letters 2 1. Physical Review Letters 1964, 13, 3–5.

(13) Ru, N.; Chu, J. H.; Fisher, I. R. Magnetic properties of the charge density wave com-pounds RTe3, R=Y, La, Ce, Pr, Nd, Sm, Gd, Tb, Dy, Ho, Er & Tm. Physical Review B 2008, 78, 4.

(14) Narsinga Rao, G.; Sankar, R.; Panneer Muthuselvam, I.; Chou, F. C. Magnetic and thermal property studies of RCrTeO6 (R=trivalent lanthanides) with layered honey-comb sublattices. Journal of Magnetism and Magnetic Materials 2014, 370, 13–17. (15) Thota, S.; Singh, K.; Nayak, S.; Simon, C.; Kumar, J.; Prellier, W. The ac-magnetic

susceptibility and dielectric response of complex spin ordering processes in Mn3O4. Journal of Applied Physics 2014, 116, 0–8.

(16) Bearpark, M. J.; Robb, M. A.; Bernardi, F.; Olivucci, M. Molecular mechanics valence bond methods for large active spaces. Application to conjugated polycyclic hydrocar-bons. Chemical Physics Letters 1994, 217, 513–519.

(17) Pauncz, R. Spin eigenfunctions: Construction and Use; PLENUM PRESS, 1979; pp XV, 370.

(18) White, R. M. Springer Series in SOLID-STATE SCIENCES ; Springer-Verlag Berlin Heidelberg, 2007; Vol. 138; p 359.

(19) Deumal, M.; Bearpark, M. J.; Novoa, J. J.; Robb, M. A. Magnetic properties of organic molecular crystals via an algebraic Heisenberg Hamiltonian. Applications to WILVIW, TOLKEK, and KAXHAS nitronyl nitroxide crystals. Journal of Physical Chemistry A 2002, 106, 1299–1315.

(20) McWeeny, R.; Sutcliffe, B. T. Methods of molecular quantum mechanics; Academic Press London, New York, 1969; pp ix, 307 p.

(21) Anderson, P. W. New Approach to the Theory of Superexchange. Physical Review 1959, 115, 1–13.

(22) Said, M.; Maynau, D.; Malrieu, J.-P.; Garcia-Bach, M. A. A nonempirical Heisenberg Hamiltonian for the study of conjugated hydrocarbons. Ground-state conformational studies. Journal of the American Chemical Society 1984, 106, 571–579.

(23) Malrieu, J.-P.; Maynau, D. A Valence Bond Effective Hamiltonian for Neutral States of π Systems. 1. Method. Journal of the American Chemical Society 1982, 104, 3021– 3029.

(24) Durand, P.; Malrieu, J.-P. Advances in Chemical Physics: Ab Initio Methods in Quan-tum Chemistry Part I ; John Wiley & Sons, Inc., 1987; Vol. 67; pp 321–412.

(25) Malrieu, J.-P. In The Concept of the Chemical Bond: Theoretical Models of Chemical Bonding Part 2 ; Maksic, Z. B., Ed.; Springer-Verlag Berlin Heidelberg, 1990; pp 107– 136.

(26) Fumanal, M.; Deumal, M. The quest for rationalizing the magnetism in purely or-ganic semiquinone-bridged bisdithiazolyl molecular magnets. Phys. Chem. Chem. Phys. 2016, 18, 20738–20749.

(27) Vela, S.; Deumal, M.; Shiga, M.; Novoa, J. J.; Ribas-Arino, J. Dynamical effects on the magnetic properties of dithiazolyl bistable materials. Chemical Science 2015, 2371– 2381.

(28) Herringer, S. N.; Deumal, M.; Ribas-Arino, J.; Novoa, J. J.; Landee, C. P.; Wikaira, J. L.; Turnbull, M. M. S=1/2 one-dimensional random-exchange ferromagnetic

zigzag ladder, which exhibits competing interactions in a critical regime. Chemistry -A European Journal 2014, 20, 8355–8362.

(29) Vela, S.; Sopena, A.; Ribas-Arino, J.; Novoa, J. J.; Deumal, M. Elucidating the 2D mag-netic topology of the ’metal-radical’ TTTA·Cu(hfac)2 system. Chemistry - A European

Journal 2014, 20, 7083–7090.

(30) Vela, S.; Deumal, M.; Ribas-Arino, J.; Novoa, J. J. Tracing the sources of the different magnetic behavior in the two phases of the bistable (BDTA)2[Co(mnt)2] compound.

Inorganic Chemistry 2012, 51, 8646–8648.

(31) Clarke, C. S.; Jornet-Somoza, J.; Mota, F.; Novoa, J. J.; Deumal, M. Origin of the magnetic bistability in molecule-based magnets: A first-principles bottom-up study of the TTTA crystal. Journal of the American Chemical Society 2010, 132, 17817–17830. (32) Deumal, M.; Rawson, J. M.; Goeta, A. E.; Howard, J. A.; Copley, R. C.; Robb, M. A.; Novoa, J. J. Studying the origin of the antiferromagnetic to spin-canting transition in the β-p-NCC6F4CNSSN· molecular magnet. Chemistry - A European Journal 2010,

16, 2741–2750.

(33) Coulson, P. C. A.; Fischer, M. I. XXXIV. Notes on the molecular orbital treatment of the hydrogen molecule. The London, Edinburgh, and Dublin Philosophical Magazine and Journal of Science 1949, 40, 386–393.

(34) Wilson, S. In Advances in the Theory of Atomic and Molecular Systems: Conceptual and Computational Advances in Quantum Chemistry; Piecuch, P., Maruani, J., Eds, S. W., Wilson, S., Eds.; 2009; Vol. 19; pp 269–294.

(35) Bearpark, M. J.; Smith, B. R.; Bernardi, F.; Olivucci, M.; Robb, M. A. Combined Quantum Mechanical and Molecular Mechanical Methods; American Chemical Society, 1998; Vol. 712; pp 148–158 SE – 9.

(36) Szabo, A.; Ostlund, N. S. Modern Quantum Chemistry: Introduction to Advanced Elec-tronic Structure Theory; Dover Books on Chemistry; Dover Publications, 1989; p 480. (37) Blancafort, L.; Celani, P.; Bearpark, M. J.; Robb, M. A. A valence-bond-based complete-active-space self-consistent-field method for the evaluation of bonding in or-ganic molecules. Theoretical Chemistry Accounts 2003, 110, 92–99.

(38) Mcweeny, R. Spins in Chemistry; Current Chemical Concepts; Academic Press London, New York, 1970; p 153.

(39) Deumal, M.; Bearpark, M. J.; Robb, M. A.; Pontillon, Y.; Novoa, J. J. The mechanism of magnetic interactions in the bulk ferromagnet para-(methylthio)phenyl nitronyl ni-troxide (YUJNEW): A first principles, bottom-up, theoretical study. Chemistry - A European Journal 2004, 10, 6422–6432.

(40) Angelini, M. C.; Parisi, G.; Ricci-Tersenghi, F. Relations between short-range and long-range Ising models. Physical Review E - Statistical, Nonlinear, and Soft Matter Physics 2014, 89, 1–11.

(41) Bera, A. K.; Yusuf, S. M.; Kumar, A.; Majumder, M.; Ghoshray, K.; Keller, L. Long-range and short-Long-range magnetic correlations, and microscopic origin of net magnetiza-tion in the spin-1 trimer chain compound CaNi3P4O14. Physical Review B 2016, 93,

1–9.

(42) Medvedev, M. V. Short-range magnetic order in a three-dimensional XXZ model with competing exchange interactions. The Physics of Metals and Metallography 2009, 107, 123–132.

(43) Hinatsu, Y.; Doi, Y. Structural phase transition and antiferromagnetic transition of Tb 3RuO7. Journal of Solid State Chemistry 2014, 220, 22–27.

(44) Aharen, T.; Greedan, J. E.; Ning, F.; Imai, T.; Michaelis, V.; Kroeker, S.; Zhou, H.; Wiebe, C. R.; Cranswick, L. M. D. Magnetic properties of the the S=3/2 geomterically frustrated double perovskites La2LiRuO6and Ba2YRuO6. Physical Review B 2009, 80,

134423.

(45) Jornet-Somoza, J.; Deumal, M.; Robb, M. A.; Landee, C. P.; Turnbul, M. M.; Feyer-herm, R.; Novoa, J. J. First-principles bottom-up study of 1D to 3D magnetic transfor-mation in the copper pyrazine dinitrate S = 1/2 antiferromagnetic crystal. Inorganic Chemistry 2010, 49, 1750–1760.

(46) Jornet, J.; Deumal, M.; Ribas-Ariño, J.; Bearpark, M. J.; Robb, M. A.; Hicks, R. G.; Novoa, J. J. Direct versus mediated through-space magnetic interactions: A first princi-ples, bottom-up reinvestigation of the magnetism of the pyridyl-verdazyl:hydroquinone molecular co-crystal. Chemistry - A European Journal 2006, 12, 3995–4005.

(47) Shapiro, A.; Landee, C. P.; Turnbull, M. M.; Jornet, J.; Deumal, M.; Novoa, J. J.; Robb, M. A.; Lewis, W. Synthesis, structure, and magnetic properties of an antiferro-magnetic spin-ladder complex: Bis(2,3-dimethylpyridinium) tetrabromocuprate. Jour-nal of the American Chemical Society 2007, 129, 952–959.

(48) Jornet-Somoza, J.; Codina-Castillo, N.; Deumal, M.; Mota, F.; Novoa, J. J.; Butcher, R. T.; Turnbull, M. M.; Keith, B.; Landee, C. P.; Wikaira, J. L. Synthe-sis, structure, magnetic behavior, and theoretical analysis of diazine-bridged magnetic ladders: Cu(quinoxoline)X2 and Cu(2,3-dimethylpyrazine)X2 (X = Cl, Br). Inorganic

Chemistry 2012, 51, 6315–6325.

(49) Vela, S.; Jornet-Somoza, J.; Turnbull, M. M.; Feyerherm, R.; Novoa, J. J.; Deumal, M. Dividing the spoils: Role of pyrazine ligands and perchlorate counterions in the mag-netic properties of bis(pyrazine)diperchloratecopper(II), [Cu(pz)2](ClO4)2. Inorganic

(50) Li, X.; Turnbull, M. M.; Landee, C. P.; Jornet, J.; Deumal, M.; Novoa, J. J.; Wikaira, J. L. Synthesis, Structure, and Magnetic Behavior of Bis(2-amino-5-fluoropyridinium) Tetrachlorocuprate(II). Inorganic Chemistry 2007, 46, 11254–11265. (51) CCDC and chemical names for the studied molecular magnets: CUP-YAR (pyrazine)dinitratocopper(II); TEXDEG bis(2,3-dimethylpyridinium) tetra-bromocuprate(II); XANKED bis(2,3-dimethylpyrazine)dihalocopper(II); CUPYZP bis(pyrazine)diperchloratecopper(II); GIVZOB bis(2-amino-5- fluoropyridinium) tetra-chlorocuprate(II); UBUBIC pyridyl-verdazyl radical:hydroquinone co-crystal; KAX-HAS p-nitrophenyl nitronyl nitroxide.

(52) Jornet-Somoza, J.; Deumal, M.; Turnbull, M. M.; Novoa, J. J. On the existence of temperature induced changes in the magnetic topology of crystals that show no first-order crystallographic phase transitions. Polyhedron 2009, 28, 1965–1971.